PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses


 Della George
 1 years ago
 Views:
Transcription
1 OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft all new document correction of RF definition and added text on failure criteria
2 OPTIMAT BLADES Page 2 of 24 TABLE OF CONTENTS 1 INTRODUCTION PREDICTION PACKAGES Classical Laminated Plate package FEM package PREDICTION OF THE UD SPECIMEN PROPERTIES Materials, layup and geometry CLT results FEM results PREDICTION OF THE MD SPECIMEN PROPERTIES Materials, layup and geometry CLT results FEM results CONCLUSION AND EVALUATION REMARKS LITERATURE...24
3 OPTIMAT BLADES Page 3 of 24 1 INTRODUCTION In this note, analysis results are given for the first analyses step in WP10. This involves predictions of the specimen strain patterns and reserve factor patterns for the Optimat Blades UD and MD specimens, using literature material data. The properties have been predicted using a CLT program and a simple FEM package. The following test cases are defined in [4]: No. type loading comments direction value [N/mm] U1t UD tension longitudinal 40 U1c UD compression longitudinal 40 U2t UD tension transverse 40 U2c UD compression transverse 40 Ust UD shear tensile tbd still to be defined M1t MD tension longitudinal 40 M1c MD compression longitudinal 40 M2t MD tension transverse 40 M2c MD compression transverse 40 Mst MD shear tensile tbd still to be defined Table 1: Load cases for the specimen predictions
4 OPTIMAT BLADES Page 4 of 24 2 PREDICTION PACKAGES 2.1 Classical Laminated Plate package The Classical Laminated Plate theory has been implemented in numerous software packages. Provided the packages have been tested thoroughly, these all should give the same results. There are some differences in the completeness of the userinterface and failure criteria offered but basically the results given are the ABD matrices, strains and stresses. The package used in this report, is a demo version of 'The Laminator' [2], a relatively easy to use and cheap package. It offers possibilities of loading the (infinite) plate and calculate the strains, stresses and socalled 'Load Vector Scale Factors'. The latter gives the ratio of fracture load and applied load. In parallel calculations have been performed with the 'Kolibri' package [1] on infinite plates. This package also has a simple finite element (see 2.2) and outputs strength results as the 'Reserve Factor' (RF) or the inverse thereof. This RF seems equivalent to the 'Load Vector Scale Factors' as used by 'The Laminator'. In this document RF will be used for both packages. 2.2 FEM package The 'Kolibri' package offers the possibility of calculating the behaviour of a finite, rectangular plate when mechanically loaded. The plate can be constrained or loaded by a uniform pressure, or a point, area or edge load. For the purpose of this investigation, and edge force has been used. The package is limited in element types: only triangular elements are possible, probably with 3 nodes (no detailed information is given). The mesh can be generated automatically, or in a regular mesh. Unfortunately it is not possible to constrain the loaded edge in such a way that global translation results. Therefore halfmodels are used (half of the specimen length) in which deformation of the cross section in the specimen middle plane is allowed although this would not occur in reality. For these reasons, the package can not be seen as a highquality FEM package like Nastran or MARC. Results can be used, however, as an illustration of the stress rise near the clamped edge. In the 'Kolibri' package three failure criteria are possible: maximum strain, maximum stress and TsaiHill. In this document only the TsaiHill criterion will be reported on.
5 OPTIMAT BLADES Page 5 of 24 3 PREDICTION OF THE UD SPECIMEN PROPERTIES 3.1 Materials, layup and geometry The material properties used for the analyses are as given for the Silenka Eglass/MY750 combination, as given in [3]. No tab material is used as there are no possibilities to model a specimen including tabs and grip constraints. For some of the material properties, the complete stressstrain curve is given, since the behaviour is nonlinear. The inplane shear properties are given in Figure 1. The actual strain at failure is 4% instead of 1.25% (when using Hooke's law). This will have some consequences for the failure load predictions. For both the CLT package applied as the FEM package, nonlinar material properties are not possible. Therefore the initial moduli will be used and the failure stress as given in [3] stress [MPa] 25 full curve Hooke strain [%] Figure 1: Stressstrain curve for inplane shear For the UD specimen a simple layup is used: 4 layers of 0 oriented layers with a thickness of 0.88 mm. The geometry of the specimen is given in [3]: a straight specimen with width of 25 mm and free length of 35 mm. The nominal specimen thickness (4 layers of material) is 3.52 mm. 3.2 CLT results Specimen stiffness and FPF strength can be predicted by the CLT package. The results are easy to describe: the specimen has the stiffness and strength properties of the UD layer itself. No layers are included with different material properties or orientation, therefore the FPF strength also is the final failure strength. The failure loads are given as running loads: force by unit width.
6 OPTIMAT BLADES Page 6 of 24 E x [MPa] E y [MPa] G xy [MPa] 5830 ν xy ν yx N xt [N/mm] N xc [N/mm] 2816 N yt [N/mm] N yc [N/mm] N xy [N/mm] Table 2: CLT results for the UD specimen layup (TsaiHill criterion) 3.3 FEM results For the FEM analyses a half model has been used, see Figure 2, of the free part of the specimen outside the grips. Although the distribution of the triangular elements is not regular, this has no significant effect on the strain distributions. Figure 2: Mesh for the UD specimen, generated automatically by the Kolibri package The rectangular plate is clamped at the left side, free at the other edges and loaded by an edge loading of 40 N/mm at the right side. Due to package limitations, no constraints on the right end are applied. The FEM package has the option to rotate the laminate. This has been used to calculate the distributions when loading the laminate in the transverse direction.
7 OPTIMAT BLADES Page 7 of 24 As can be seen from the strain distributions in Figure 4, at the loaded end the specimen is not strained homogenously. This is a consequence of the short free length of the specimen. For a specimen with doubled length strains are homogeneous at the loaded end, as can be seen in Figure 3. It should be noted that the strain distributions over the first 17.5mm from the clamped side are not the same for both models. Figure 3: Longitudinal strain distribution for double length (load case U1t) The predicted patterns of the strain and the inverse of the reserve factor are given in Figure 4 to Figure 9. Peak strains always occur at the corners of the clamped side of the specimen, as can be expected. The strain values itself are also influenced by the number of elements used in the mesh. Smaller elements apparently lead to higher peak strain values. For tensile loaded cases, the inverse of the reserve factor per layer is dominated by the strain transverse to the fibre. For compression loaded cases, domination is less simple. ε x strains [%] ε y 1/RF CLT max CLT max CLT max M1t M1c M2t M2c Table 3: Strains and strength aspects of UD specimen Values for the strains and the inverse of the reserve factors, for a loading of 40 N/mm, are given in Table 3 for an infinite plate (designated 'CLT') and the extreme values for the FEM
8 OPTIMAT BLADES Page 8 of 24 models. As can be seen from the table, the peak strains in the specimen are predicted considerably higher than for an infinite pate. As a consequence, the margin to failure is much smaller.
9 OPTIMAT BLADES Page 9 of 24 Figure 4: Laminate strain distributions at load case U1t (Fx = 40 N/mm)
10 OPTIMAT BLADES Page 10 of 24 Figure 5: Reserve factor distributions for the 0 layer at load case U1t Figure 6: Reserve factor distributions for the 0 layer at load case U1c (Fx = 40 N/mm)
11 OPTIMAT BLADES Page 11 of 24 Figure 7: Laminate strain distributions at load case U2t (Fy = 40 N/mm)
12 OPTIMAT BLADES Page 12 of 24 Figure 8: Reserve factor distributions for the 0 layer at load case U2t Figure 9: Reserve factor distributions for the 0 layer at load case U2c (Fy = 40 N/mm)
13 OPTIMAT BLADES Page 13 of 24 4 PREDICTION OF THE MD SPECIMEN PROPERTIES 4.1 Materials, layup and geometry The material properties used for the analyses are as given for the Silenka Eglass/MY750 combination, as given in [3]. No tab material is used as there are no possibilities to model a specimen including tabs and grip constraints. For the MD specimen [3] a 14layer layup is used: 4 layers of 0 oriented layers with a thickness of 0.88 mm and 10 layers of 45 oriented layers with a thickness of 0.88 mm. The total layup is: (45/45/0/45/45/0/45/45/0/45/45/0/45/45). The layup is therefore not symmetrical. The geometry of the specimen is given in [3]: a straight specimen with width of 25 mm, free length of 40 mm and thickness of 6.57 mm. 4.2 CLT results The evaluated laminate is nonsymmetrical, therefore the strains in all layers with the same fibre orientation may differ. Nonzero values can be found in the Bmatrix in positions B 16 and B 26. The stiffness properties for the laminate and the laminate FPF uniaxial strengths, according to the TsaiHill failure criterion, are given in Table 4. E x [MPa] E y [MPa] G xy [MPa] 9419 ν xy ν yx N xt [N/mm] N xc [N/mm] N yt [N/mm] N yc [N/mm] N xy [N/mm] Table 4: CLT results for the MD specimen layup (TsaiHill criterion) For the load cases, as given in Table 1, different failure criteria can be compared. The results for the maximum stress, TsaiHill and TsaiWu criteria are given in Table 5. In general the differences are small for the plates in tension and shear loading. Larger differences occur for the compression loaded plates, especially for the 0 degree layer in transverse compression. In view of the large differences between the reserve factors for the 0 and 45 layer in e.g. load case 'xt', the final failure can be expected to be at a much higher load. Even more so, since the stressstrain behaviour of the 45 layer is clearly nonlinear at higher stress levels.
14 OPTIMAT BLADES Page 14 of 24 Maximum stress TsaiHill TsaiWu layer xt xc yt yc xy Table 5: Reserve factors at 40 N/mm applied load (MD specimen layup) 4.3 FEM results For the FEM analyses a half model has been used, see Figure 10. Although the distribution of the triangular elements is not regular, this has no significant effect on the strain distributions that will be shown later. Figure 10: Mesh for the MD specimen, generated automatically by the Kolibri package The rectangular plate is clamped at the left side and loaded by an edge loading of 40 N/mm at the right side. Due to package limitations, no constraints on the right end are applied. A quarter model gave slightly different results as a result of the nonsymmetrical laminate. The deformed shape for load case M1t is given in Figure 11. It clearly shows the effect of the nonsymmetrical layup
15 OPTIMAT BLADES Page 15 of 24 Figure 11: Deformed shape of the MD specimen for load case M1t The predicted patterns of the strain and the inverse of the reserve factor are given in Figure 13 to Figure 18. As can be seen in most of the transverse strain graphs (see e.g. lower graph of Figure 13) the strain at the specimen free end is not yet homogeneous. This is a result of the relative short specimen free length chosen in the project. For a specimen with twice the free length (i.e. 80 mm) the strain distribution at the middle section would be close to homogenous, see Figure 12 for load case M1t.
16 OPTIMAT BLADES Page 16 of 24 Figure 12: Transverse strain distribution for a model with double length Peak strains always occur at the corners of the clamped side of the specimen, as can be expected. The strain values itself are also influenced by the number of elements used in the mesh. Smaller elements apparently lead to higher peak strain values. As was the case for the UD specimen, for tensile loaded cases the inverse of the reserve factor per layer is clearly dominated by the strain transverse to the fibre. For compression loaded cases no simple relationship is possible between a strain component and the strength. strains [%] 1/RF ε x ε y 45 layer 0 layer CLT max CLT max CLT max CLT max M1t M1c M2t M2c Table 6: Strains and strength aspects of MD specimen Values for the strains and the inverse of the reserve factors, for a loading of 40 N/mm, are given in Table 6 for an infinite plate (designated 'CLT') and the extreme values for the FEM models. As can be seen from the table, the peak strains in the specimen are predicted considerably higher than for an infinite pate. As a consequence, the margin to failure is much smaller.
17 OPTIMAT BLADES Page 17 of 24 Figure 13: Laminate strain distributions at load case M1t (Fx = 40 N/mm)
18 OPTIMAT BLADES Page 18 of 24 Figure 14: Reserve factor distributions for 45 layer (top) and 0 layer (bottom) at load case M1t
19 OPTIMAT BLADES Page 19 of 24 Figure 15: Reserve factor distributions for 45 layer (top) and 0 layer (bottom) at load case M1c (Fx = 40 N/mm)
20 OPTIMAT BLADES Page 20 of 24 Figure 16: Laminate strain distributions at load case M2t (Fy = 40 N/mm)
21 OPTIMAT BLADES Page 21 of 24 Figure 17: Reserve factor distributions for 45 layer (top) and 0 layer (bottom) at load case M2t
22 OPTIMAT BLADES Page 22 of 24 Figure 18: Reserve factor distributions for 45 layer (top) and 0 layer (bottom) at load case M2c (Fy = 40 N/mm)
23 OPTIMAT BLADES Page 23 of 24 5 CONCLUSION AND EVALUATION REMARKS Mechanical properties have been calculated for two standard Optimat Blades test specimens, on basis of assumed material properties. The stiffness and firstplyfailure strength of an infinite plate has been predicted using the Classical Laminated plate theory for linear stressstrain relationships. For the MD specimen, three failure theories have been applied: maximum stress, TsaiHill and TsaiWu. For tensile and shear loaded MD plates, the differences between the theories is small. For compression loaded plates, TsaiWu predicts higher strengths for the 45 layer and (for Xc) significantly lower strengths for the 0 layer. The FEM package used is limited in many respects, therefore the results are seen as first order approximations only. Peak stresses (or strains) are in all cases expected at the clamped end of the specimen (at the grip). The specimen length is relatively small, therefore the strains are not expected to be homogeneous in the specimen middle. Due to the high peak stresses near the grips, the predicted strength of the specimen is much smaller than the values given for the infinite plate, sometimes by a factor of 23. The MD specimen is defined as nonsymmetrical. This complicates simple modelling of the specimen. The builtup of the MD specimen has to be checked.
24 OPTIMAT BLADES Page 24 of 24 6 LITERATURE [1] Kolibri package, Kolibri Evaluation Edition, CLC TU DelftTNO, the Netherlands, see [2] 'The Laminator', version 3.1, see [3] Joosse, P.A.: "Laminae and specimen definitions for FEM analyses TG4"; TU Delft, WMCGroup, doc. OB_TG4_N002 rev2, [4] Joosse, P.A.: "Proposal for the first analysis step for WP10"; TU Delft, WMCGroup, doc. OB_TG4_N003,
QUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationGetting Started with Composites Modeling and Analysis
Getting Started with Composites Modeling and Analysis IN THIS WEBINAR: PRESENTED BY: Orthotropic materials and how to define them Composite Laminate properties and modeling Composite failure theories and
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationACDC. User Manual. Ver. 1.0
ACDC User Manual Ver. 1.0 Centre Composite December 2016 ACDC, Ver. 1.0 User Manual Centre Composite, 2016 (software@composite.lv) Table of Contents Introduction... 1 System requirements... 1 Theoretical
More informationINTERNATIONAL JOURNAL OF APPLIED ENGINEERING RESEARCH, DINDIGUL Volume 2, No 1, 2011
Interlaminar failure analysis of FRP cross ply laminate with elliptical cutout Venkateswara Rao.S 1, Sd. Abdul Kalam 1, Srilakshmi.S 1, Bala Krishna Murthy.V 2 1 Mechanical Engineering Department, P. V.
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationTABLE OF CONTENTS. Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA TABLE OF CONTENTS 1. INTRODUCTION TO COMPOSITE MATERIALS 1.1 Introduction... 1.2 Classification... 1.2.1
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationModelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations
Modelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations W. Van Paepegem *, I. De Baere and J. Degrieck Ghent
More informationPURE BENDING. If a simply supported beam carries two point loads of 10 kn as shown in the following figure, pure bending occurs at segment BC.
BENDING STRESS The effect of a bending moment applied to a crosssection of a beam is to induce a state of stress across that section. These stresses are known as bending stresses and they act normally
More informationComparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost
Comparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost 1 Mihir A. Mehta, 2 Satyen D. Ramani 1 PG Student, Department
More informationAERSYS KNOWLEDGE UNIT
7016 1. INTRODUCTION The scope of this document is to provide a clarification and a deeper understanding of the two different ways to move the mid plane of the element out of the nodal plane. Although
More informationStrength Prediction Of Composite Laminate
Strength Prediction Of Composite te Prof. Yogananda. A 1, Mr. R. Vijayakumar 2 Assistant Professor, Department of Mechanical Engineering, East West Institute of Technology, Bangalore. Research Scholar,
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationFinite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix)
Finite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix) Nikhil J. Chaudhari 1 Post Graduate Student Department of Mechanical Engineering Veermata Jijabai Technological Institute
More informationNORMAL STRESS. The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts.
NORMAL STRESS The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts. σ = force/area = P/A where σ = the normal stress P = the centric
More informationNUMERICAL SIMULATION OF DAMAGE IN THERMOPLASTIC COMPOSITE MATERIALS
5 th European LSDYNA Users Conference Composites NUMERICAL SIMULATION OF DAMAGE IN THERMOPLASTIC COMPOSITE MATERIALS Kevin Brown 1, Richard Brooks, Nicholas Warrior School of Mechanical, Materials and
More informationDYNAMIC FAILURE ANALYSIS OF LAMINATED COMPOSITE PLATES
Association of Metallurgical Engineers of Serbia AMES Scientific paper UDC:669.1419:628.183=20 DYNAMIC FAILURE ANALYSIS OF LAMINATED COMPOSITE PLATES J. ESKANDARI JAM 1 and N. GARSHASBI NIA 2 1 Aerospace
More informationSKINSTRINGER DEBONDING AND DELAMINATION ANALYSIS IN COMPOSITE STIFFENED SHELLS
SKINSTRINER DEBONDIN AND DELAMINATION ANALYSIS IN COMPOSITE STIFFENED SHELLS R. Rikards, K. Kalnins & O. Ozolinsh Institute of Materials and Structures, Riga Technical University, Riga 1658, Latvia ABSTRACT
More informationAn orthotropic damage model for crash simulation of composites
High Performance Structures and Materials III 511 An orthotropic damage model for crash simulation of composites W. Wang 1, F. H. M. Swartjes 1 & M. D. Gan 1 BU Automotive Centre of Lightweight Structures
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationOpenhole compressive strength prediction of CFRP composite laminates
Openhole compressive strength prediction of CFRP composite laminates O. İnal 1, A. Ataş 2,* 1 Department of Mechanical Engineering, Balikesir University, Balikesir, 10145, Turkey, inal@balikesir.edu.tr
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationEffect of Thermal Stresses on the Failure Criteria of Fiber Composites
Effect of Thermal Stresses on the Failure Criteria of Fiber Composites Martin Leong * Institute of Mechanical Engineering Aalborg University, Aalborg, Denmark Bhavani V. Sankar Department of Mechanical
More informationCalibration and Experimental Validation of LSDYNA Composite Material Models by Multi Objective Optimization Techniques
9 th International LSDYNA Users Conference Optimization Calibration and Experimental Validation of LSDYNA Composite Material Models by Multi Objective Optimization Techniques Stefano Magistrali*, Marco
More informationEXPLICIT DYNAMIC SIMULATION OF DROPWEIGHT LOW VELOCITY IMPACT ON CARBON FIBROUS COMPOSITE PANELS
EXPLICIT DYNAMIC SIMULATION OF DROPWEIGHT LOW VELOCITY IMPACT ON CARBON FIBROUS COMPOSITE PANELS Umar Farooq and Karl Gregory School of Built Environment and Department of Engineering, University of Bolton,
More informationA HIGHERORDER BEAM THEORY FOR COMPOSITE BOX BEAMS
A HIGHERORDER BEAM THEORY FOR COMPOSITE BOX BEAMS A. Kroker, W. Becker TU Darmstadt, Department of Mechanical Engineering, Chair of Structural Mechanics Hochschulstr. 1, D64289 Darmstadt, Germany kroker@mechanik.tudarmstadt.de,
More informationMICROMECHANICAL ANALYSIS OF FRP COMPOSITES SUBJECTED TO LONGITUDINAL LOADING
MICROMECHANICAL ANALYSIS OF FRP COMPOSITES SUBJECTED TO LONGITUDINAL LOADING N. Krishna Vihari 1, P. Phani Prasanthi 1, V. Bala Krishna Murthy 2* and A. Srihari Prasad 3 1 Mech. Engg. Dept., P. V. P. Siddhartha
More informationDAMAGE MECHANICS MODEL FOR OFFAXIS FATIGUE BEHAVIOR OF UNIDIRECTIONAL CARBON FIBERREINFORCED COMPOSITES AT ROOM AND HIGH TEMPERATURES
DAMAGE MECHANICS MODEL FOR OFFAXIS FATIGUE BEHAVIOR OF UNIDIRECTIONAL CARBON FIBERREINFORCED COMPOSITES AT ROOM AND HIGH TEMPERATURES M. Kawai Institute of Engineering Mechanics University of Tsukuba,
More informationAs an example we consider the stacking and analysis of a 2ply symmetric laminate. First we clear the Matlab space and close figures.
Program Lam 1 Introduction The collection of Matlab command and function files in the package lam allows the stacking and analysis of a laminate. In fact only a representative piece of a laminate is considered,
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationAn investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More informationSamantha Ramirez, MSE. Stress. The intensity of the internal force acting on a specific plane (area) passing through a point. F 2
Samantha Ramirez, MSE Stress The intensity of the internal force acting on a specific plane (area) passing through a point. Δ ΔA Δ z Δ 1 2 ΔA Δ x Δ y ΔA is an infinitesimal size area with a uniform force
More informationCHAPTER 3 THE EFFECTS OF FORCES ON MATERIALS
CHAPTER THE EFFECTS OF FORCES ON MATERIALS EXERCISE 1, Page 50 1. A rectangular bar having a crosssectional area of 80 mm has a tensile force of 0 kn applied to it. Determine the stress in the bar. Stress
More informationPredicting Failure of Multiangle Composite Laminates
Predicting Failure of Multiangle Composite Laminates Preliminary discussion (not in textbook): Micromechanics failure analyses vs Macromechanics failure analyses Fiber Architecture of Some Common Composite
More information6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa ( psi) and
6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original diameter of 3.8 mm (0.15 in.) will experience only elastic deformation when a tensile
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationMASONRY MICROMODELLING ADOPTING A DISCONTINUOUS FRAMEWORK
MASONRY MICROMODELLING ADOPTING A DISCONTINUOUS FRAMEWORK J. PinaHenriques and Paulo B. Lourenço School of Engineering, University of Minho, Guimarães, Portugal Abstract Several continuous and discontinuous
More informationMultiscale Approach to Damage Analysis of Laminated Composite Structures
Multiscale Approach to Damage Analysis of Laminated Composite Structures D. Ivančević and I. Smojver Department of Aeronautical Engineering, Faculty of Mechanical Engineering and Naval Architecture, University
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationFig. 1. Different locus of failure and crack trajectories observed in mode I testing of adhesively bonded double cantilever beam (DCB) specimens.
a). Cohesive Failure b). Interfacial Failure c). Oscillatory Failure d). Alternating Failure Fig. 1. Different locus of failure and crack trajectories observed in mode I testing of adhesively bonded double
More informationPREDICTION OF BUCKLING AND POSTBUCKLING BEHAVIOUR OF COMPOSITE SHIP PANELS
FONDATĂ 1976 THE ANNALS OF DUNAREA DE JOS UNIVERSITY OF GALATI. FASCICLE IX. METALLURGY AND MATERIALS SCIENCE N 0. 007, ISSN 15 08X PREDICTION OF BUCKLING AND POSTBUCKLING BEHAVIOUR OF COMPOSITE SHIP PANELS
More informationAnalysis of Composite Pressure Vessels
Analysis of Composite Pressure Vessels Reza Mohammadzadeh Gheshlaghi 1 Mohammad Hassan Hojjati Hamid Reza Mohammadi Daniali 3 1 Engineering Research Centre, Tabriz, Iran,3 Department of Mechanical Engineering,
More informationStatic and Time Dependent Failure of Fibre Reinforced Elastomeric Components. Salim Mirza Element Materials Technology Hitchin, UK
Static and Time Dependent Failure of Fibre Reinforced Elastomeric Components Salim Mirza Element Materials Technology Hitchin, UK Introduction Fibre reinforced elastomers are used in many applications,
More informationLSDYNA MAT54 for simulating composite crash energy absorption
LSDYNA MAT54 for simulating composite crash energy absorption Bonnie Wade and Paolo Feraboli (UW) Mostafa Rassaian (Boeing BR&T) JAMS 2011 The Joint Advanced Materials and Structures Center of Excellence
More informationSIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO MULTIPLE LOADING WITH MEMBRANEFLEXION COUPLING EFFECTS
VOL. 5, NO. 4, APRIL 010 ISSN 18196608 006010 Asian Research Publishing Network (ARPN). All rights reserved. SIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO
More informationPractice Final Examination. Please initial the statement below to show that you have read it
EN175: Advanced Mechanics of Solids Practice Final Examination School of Engineering Brown University NAME: General Instructions No collaboration of any kind is permitted on this examination. You may use
More informationNUMERICAL FEM ANALYSIS FOR THE PART OF COMPOSITE HELICOPTER ROTOR BLADE
Journal of KONES Powertrain and Transport, Vol. 19, No. 1 2012 NUMERICAL FEM ANALYSIS FOR THE PART OF COMPOSITE HELICOPTER ROTOR BLADE Hubert D bski Lublin University of Technology, Department of Machine
More informationTRIALS WITH A SIMPLIFIED METHOD FOR BUCKLING AND ULTIMATE STRENGTH ANALYSIS OF COMPOSITE PLATES
DEPT. OF MATH., UNIVERSITY OF OSLO RESEARCH REPORT IN MECHANICS, No. 1 ISSN 08019940 December 2012 TRIALS WITH A SIMPLIFIED METHOD FOR BUCKLING AND ULTIMATE STRENGTH ANALYSIS OF COMPOSITE PLATES by Qiao
More informationFailure from static loading
Failure from static loading Topics Quiz /1/07 Failures from static loading Reading Chapter 5 Homework HW 3 due /1 HW 4 due /8 What is Failure? Failure any change in a machine part which makes it unable
More informationComputational Analysis for Composites
Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics
More informationEffect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test
Effect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test M. Praveen Kumar 1 and V. Balakrishna Murthy 2* 1 Mechanical Engineering Department, P.V.P. Siddhartha Institute of Technology,
More informationCapability Assessment of Finite Element Software in Predicting the Last Ply Failure of Composite Laminates
Available online at www.sciencedirect.com Procedia Engineering 41 (2012 ) 1647 1653 International Symposium on Robotics and Intelligent Sensors 2012 (IRIS 2012) Capability Assessment of Finite Element
More informationStructural behaviour of traditional mortiseandtenon timber joints
Structural behaviour of traditional mortiseandtenon timber joints Artur O. Feio 1, Paulo B. Lourenço 2 and José S. Machado 3 1 CCR Construtora S.A., Portugal University Lusíada, Portugal 2 University
More informationSmart Materials, Adaptive Structures, and Intelligent Mechanical Systems
Smart Materials, Adaptive Structures, and Intelligent Mechanical Systems Bishakh Bhattacharya & Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 19 Analysis of an Orthotropic Ply References
More informationComposite FEM Labwork
Composite FEM Labwork You may perform these exercises in groups of max 2 persons. You may also between exercise 5 and 6. Be critical on the results obtained! Exercise 1. Open the file exercise1.inp in
More informationNumerical Analysis of Composite Panels in the PostBuckling Field taking into account Progressive Failure
Copyright c 007 ICCES ICCES, vol.1, no.3, pp.9398, 007 Numerical Analysis of Composite Panels in the PostBuckling Field taking into account Progressive Failure C. Bisagni 1 Summary The research here
More information15 INTERLAMINAR STRESSES
15 INTERLAMINAR STRESSES 151 OUTOFPLANE STRESSES Classical laminate plate theor predicts the stresses in the plane of the lamina,, and τ but does not account for outofplane stresses, τ and τ. It assumes
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationFailure analysis of serial pinned joints in composite materials
Indian Journal of Engineering & Materials Sciences Vol. 18, April 2011, pp. 102110 Failure analysis of serial pinned joints in composite materials Alaattin Aktaş* Department of Mechanical Engineering,
More information9 Strength Theories of Lamina
9 trength Theories of Lamina 9 TRENGTH O ORTHOTROPIC LAMINA or isotropic materials the simplest method to predict failure is to compare the applied stresses to the strengths or some other allowable stresses.
More informationME 7502 Lecture 2 Effective Properties of Particulate and Unidirectional Composites
ME 75 Lecture Effective Properties of Particulate and Unidirectional Composites Concepts from Elasticit Theor Statistical Homogeneit, Representative Volume Element, Composite Material Effective Stress
More informationComposite Laminate Modeling
omposite Laminate Modeling White Paper for Femap and NX Nastran Users Venkata Bheemreddy, Ph.D., Senior Staff Mechanical Engineer Adrian Jensen, PE, Senior Staff Mechanical Engineer WHAT THIS WHITE PAPER
More informationThe influence of fiber undulation on the mechanical properties of FRPlaminates. Christian Fiebig, Michael Koch
URN (Paper): urn:nbn:de:gbv:ilm12014iwk099:3 58 th ILMENAU SCIENTIFIC COLLOQUIUM Technische Universität Ilmenau, 08 12 September 2014 URN: urn:nbn:de:gbv:ilm12014iwk:3 The influence of fiber undulation
More informationCOMPARISON OF NUMERICAL SIMULATION AND EXPERIMENT OF A FLEXIBLE COMPOSITE CONNECTING ROD
10th International DAAAM Baltic Conference "INDUSTRIAL ENGINEERING  1213 May 2015, Tallinn, Estonia COMPARISON OF NUMERICAL SIMULATION AND EXPERIMENT OF A FLEXIBLE COMPOSITE CONNECTING ROD Sedláček,
More informationMulti Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala
Multi Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala Abstract: FRP laminated composites have been extensively used in Aerospace and allied industries
More informationA Stress Gradient Failure Theory for Textile Structural Composites. Final Technical Report submitted to ARO
A Stress Gradient Failure Theory for Textile Structural Composites Final Technical Report submitted to ARO By RYAN KARKKAINEN and BHAVANI SANKAR University of Florida Department of Mechanical & Aerospace
More informationIntroduction to Aerospace Engineering
Introduction to Aerospace Engineering Lecture slides Challenge the future 1 Aircraft & spacecraft loads Translating loads to stresses Faculty of Aerospace Engineering 29112011 Delft University of Technology
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationExample3. Title. Description. Cylindrical Hole in an Infinite MohrCoulomb Medium
Example3 Title Cylindrical Hole in an Infinite MohrCoulomb Medium Description The problem concerns the determination of stresses and displacements for the case of a cylindrical hole in an infinite elastoplastic
More informationFinite element analysis of drilled holes in unidirectional composite laminates using failure theories
American Journal of Science and Technology 2014; 1(3): 101105 Published online May 30, 2014 (http://www.aascit.org/journal/ajst) Finite element analysis of drilled holes in unidirectional composite laminates
More informationPREDICTION OF OUTOFPLANE FAILURE MODES IN CFRP
PREDICTION OF OUTOFPLANE FAILURE MODES IN CFRP R. R. Pinto 1, P. P. Camanho 2 1 INEGI  Instituto de Engenharia Mecanica e Gestao Industrial, Rua Dr. Roberto Frias, 4200465, Porto, Portugal 2 DEMec,
More informationLaboratory 4 Bending Test of Materials
Department of Materials and Metallurgical Engineering Bangladesh University of Engineering Technology, Dhaka MME 222 Materials Testing Sessional.50 Credits Laboratory 4 Bending Test of Materials. Objective
More informationPROGRESSIVE DAMAGE ANALYSES OF SKIN/STRINGER DEBONDING. C. G. Dávila, P. P. Camanho, and M. F. de Moura
PROGRESSIVE DAMAGE ANALYSES OF SKIN/STRINGER DEBONDING C. G. Dávila, P. P. Camanho, and M. F. de Moura Abstract The debonding of skin/stringer constructions is analyzed using a stepbystep simulation
More informationEDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES AND APPLICATIONS NQF LEVEL 3 OUTCOME 1  LOADING SYSTEMS TUTORIAL 3 LOADED COMPONENTS
EDEXCEL NATIONAL CERTIICATE/DIPLOMA MECHANICAL PRINCIPLES AND APPLICATIONS NQ LEVEL 3 OUTCOME 1  LOADING SYSTEMS TUTORIAL 3 LOADED COMPONENTS 1. Be able to determine the effects of loading in static engineering
More informationNumerical modeling of standard rock mechanics laboratory tests using a finite/discrete element approach
Numerical modeling of standard rock mechanics laboratory tests using a finite/discrete element approach S. Stefanizzi GEODATA SpA, Turin, Italy G. Barla Department of Structural and Geotechnical Engineering,
More informationCrash and Impact Simulation of Composite Structures by Using CAE Process Chain
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de
More informationFracture Mechanics, Damage and Fatigue: Composites
University of Liège Aerospace & Mechanical Engineering Fracture Mechanics, Damage and Fatigue: Composites Ludovic Noels Computational & Multiscale Mechanics of Materials CM3 http://www.ltascm3.ulg.ac.be/
More informationModeling and Simulations of Aircraft Structures Stiffness, Damage, and Failure Prediction for Laminated Composites
Modeling and Simulations of Aircraft Structures Stiffness, Damage, and Failure Prediction for Laminated Composites H.E.Pettermann 1, C.Schuecker 1, D.H.Pahr 2, F.G.Rammerstorfer 2 1 Austrian Aeronautics
More informationStress, Strain Stress strain relationships for different types of materials Stress strain relationships for a unidirectional/bidirectional lamina
Chapter 2 Macromechanical Analysis of a Lamina Stress, Strain Stress strain relationships for different types of materials Stress strain relationships for a unidirectional/bidirectional lamina Islamic
More informationAn overview of Carbon Fiber modeling in LSDYNA. John Zhao October 23 th 2017
An overview of Carbon Fiber modeling in LSDYNA John Zhao zhao@lstc.com October 23 th 2017 Outline Manufacturing of Carbon Fiber Compression molding *MAT_277 & 278 *MAT_293 *MAT_249 Resin transform molding
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 15 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationMECHANICS OF MATERIALS
00 The McGrawHill Companies, Inc. All rights reserved. T Edition CHAPTER MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Teas Tech Universit
More informationEFFECTIVITY PAGE DATE ISSUE PAGE DATE ISSUE PAGE DATE ISSUE 24/07/14 24/07/14
173 ROCHEFORT FAX: (33) 5 46 87 4 12 EFFECTIVITY PAGE DATE ISSUE PAGE DATE ISSUE PAGE DATE ISSUE 1 2 3 4 5 6 7 8 9 1 11 12 13 14 15 16 17 18 19 2 21 22 23 24 25 26 27 28 29 3 24/7/14 24/7/14 24/7/14 24/7/14
More informationTable of Contents. Preface...xvii. Part 1. Level
Preface...xvii Part 1. Level 1... 1 Chapter 1. The Basics of Linear Elastic Behavior... 3 1.1. Cohesion forces... 4 1.2. The notion of stress... 6 1.2.1. Definition... 6 1.2.2. Graphical representation...
More informationUniversity of Sheffield The development of finite elements for 3D structural analysis in fire
The development of finite elements for 3D structural analysis in fire Chaoming Yu, I. W. Burgess, Z. Huang, R. J. Plank Department of Civil and Structural Engineering StiFF 05/09/2006 3D composite structures
More informationOptimum Height of Plate Stiffener under Pressure Effect
The st Regional Conference of Eng. Sci. NUCEJ Spatial ISSUE vol., No.3, 8 pp 459468 Optimum Height of Plate Stiffener under Pressure Effect Mazin Victor Yousif M.Sc Production Engineering University of
More informationComposite models 30 and 131: Ply types 0 and 8 calibration
Model calibration Composite BiPhase models 30 and 3 for elastic, damage and failure PAMCRASH material model 30 is for solid and 3 for multilayered shell elements. Within these models different ply types
More informationStrength of GRPlaminates with multiple fragment damages
Strength of GRPlaminates with multiple fragment damages S. Kazemahvazi, J. Kiele, D. Zenkert Kungliga Tekniska Högskolan, KTH 100 44 Stockholm, Sweden sohrabk@kth.se SUMMARY The strength of glass fibre
More informationAutomatic Buckling Checks on Stiffened Panels Based on Finite Element Results
Delft University of Technology Faculty of Civil Engineering & Geosciences Department of Structural Mechanics Automatic Buckling Checks on Stiffened Panels Based on Finite Element Results Master Thesis
More informationCoupling of plasticity and damage in glass fibre reinforced polymer composites
EPJ Web of Conferences 6, 48 1) DOI: 1.151/epjconf/1648 c Owned by the authors, published by EDP Sciences, 1 Coupling of plasticity and damage in glass fibre reinforced polymer composites R. Kvale Joki
More informationDAMAGE SIMULATION OF CFRP LAMINATES UNDER HIGH VELOCITY PROJECTILE IMPACT
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS DAMAGE SIMULATION OF CFRP LAMINATES UNDER HIGH VELOCITY PROJECTILE IMPACT A. Yoshimura 1*, T. Okabe, M. Yamada 3, T. Ogasawara 1, Y. Tanabe 3 1 Advanced
More informationFinite Element Method in Geotechnical Engineering
Finite Element Method in Geotechnical Engineering Short Course on + Dynamics Boulder, Colorado January 58, 2004 Stein Sture Professor of Civil Engineering University of Colorado at Boulder Contents Steps
More informationCHAPTER THREE SYMMETRIC BENDING OF CIRCLE PLATES
CHAPTER THREE SYMMETRIC BENDING OF CIRCLE PLATES * Governing equations in beam and plate bending ** Solution by superposition 1.1 From Beam Bending to Plate Bending 1.2 Governing Equations For Symmetric
More informationAfter lecture 16 you should be able to
Lecture 16: Design of paper and board packaging Advanced concepts: FEM, Fracture Mechanics After lecture 16 you should be able to describe the finite element method and its use for paper based industry
More informationCalculation of Damagedependent Directional Failure Indices from the TsaiWu Static Failure Criterion
Van Paepegem, W. and Degrieck, J. (3. alculation of Damagedependent Directional Failure Indices from the saiwu Static Failure riterion. omposites Science and echnology, 63(, 353. alculation of Damagedependent
More informationModelling the behaviour of plastics for design under impact
Modelling the behaviour of plastics for design under impact G. Dean and L. Crocker MPP IAG Meeting 6 October 24 Land Rover door trim Loading stages and selected regions Project MPP7.9 Main tasks Tests
More information